# Research Article Thermo Elastic-Plastic Analysis of Rotating 2019-07-31¢ ermo...

date post

19-Mar-2020Category

## Documents

view

2download

0

Embed Size (px)

### Transcript of Research Article Thermo Elastic-Plastic Analysis of Rotating 2019-07-31¢ ermo...

Hindawi Publishing Corporation Advances in Materials Science and Engineering Volume 2013, Article ID 810508, 11 pages http://dx.doi.org/10.1155/2013/810508

Research Article Thermo Elastic-Plastic Analysis of Rotating Functionally Graded Stainless Steel Composite Cylinder under Internal and External Pressure Using Finite Difference Method

Sanjeev Sharma and Sanehlata Yadav

Department of Mathematics, Jaypee Institute of Information Technology, A-10, Sector 62, Noida, Uttar Pradesh 201307, India

Correspondence should be addressed to Sanjeev Sharma; sanjeev.sharma@jiit.ac.in

Received 22 July 2013; Accepted 26 October 2013

Academic Editor: Mohd Sapuan Salit

Copyright © 2013 S. Sharma and S. Yadav. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

The thermal elastic-plastic stresses have been investigated for a rotating functionally graded stainless steel composite cylinder under internal and external pressure with general nonlinear strain hardening law and von Mises’ yield criterion using finite difference method. The modulus of elasticity in the rotating cylinder varies radially according to power law and the temperature distribution satisfies Laplace heat equation in radial direction. From the analysis, we can conclude that cylindermade of functionally graded stainless steel composite material with variable thickness and variable density under thermal loading for Swift’s strain hardening measure 𝑚 = 0.6 is better choice of the design as compared to homogeneous cylinder. This is because of the reason that circumferential stress is less for functionally graded stainless steel composite cylinder as compared to homogeneous cylinder for Swift’s strain hardening measure 𝑚 = 0.6 under internal and external pressure. This leads to the idea of “stress saving” which minimizes the possibility of fracture of cylinder.

1. Introduction

Thermo elastic-plastic analysis of functionally graded mate- rials under internal and external pressure is an active topic for engineering mechanics. The study of thick-walled cylinder is an interesting area of research and highly used due to vast utilization in the pressure vessels and pipes and so forth. Functionally graded materials are nothing but nonhomogeneous composite materials which are highly heat resistant and very promising in high-tech engineering fields [1, 2]. The demands of functionally graded materials are increasing under high rotation and temperature. These materials find their applications in many areas, that is, flywheels, aerospace, nuclear reactors, compressors, and so forth. The problems of rotating thick-walled cylinder and plates can be found in many text books of elasticity [3, 4]. Obata et al. [5] calculated stresses for a hollow circular cylinder and hollow sphere under thermal loading using perturbation method. For these materials they found that

the perturbation solutions had good convergence. Perry and Aboudi [6] calculated the residual stresses in a homogeneous cylinder using finite difference method and concluded that it is very effective in solving autofrettage problem numer- ically. Gao [7] investigated elastic-plastic stresses, strains, and displacements in a cylinder under internal pressure using elastic strain hardening in the plane strain conditions. Tutuncu and Ozturk [8] studied the closed form solution for stresses and displacement in cylindrical and spherical vessels made of functionally graded material subjected to internal pressure using infinitesimal theory of elasticity.They compared stress distributions in functionally gradedmaterial with homogeneous material. Singh and Gupta [9] developed a mathematical model to describe steady-state creep in an isotropic functionally graded composite subjected to internal pressure which contains linearly varying silicon carbide particles in a matrix of pure aluminum. They observed that the radial stress in the cylinder decreases throughout with the increase in reinforcement gradient, whereas the tangential,

2 Advances in Materials Science and Engineering

axial, and effective stresses increase significantly near the inner radius but show significant decrease towards the outer radius. Aggarwal et al. [10] investigated safety factors in terms of elastic-plastic stresses for functionally graded thick- walled circular cylinder under internal and external pressure and concluded that functionally graded thick-walled cylinder minimizes the possibility of fracture of the cylinder. Aggarwal et al. [11] calculated thermal creep stresses for nonhomo- geneous thick-walled cylinder under internal and external pressure using Lebesgue strain measure and concluded that nonhomogeneous cylinder is better choice of design as compared to homogeneous cylinder. Parvizi et al. [12] studied amathematicalmodel to predict the yielding in a functionally graded Al A359/SiCp cylinder and find closed form solution for plastic stresses using Tresca’s yield criterion subjected to internal pressure with thermal loading. They observed that there is a point in cylinder where the hoop stress changes from compressive to tensile and the position of this point is independent of the temperature gradient and depends on material properties and geometry of the functionally graded cylinder. Eraslan and Akgül [13] calculated the numerical solution for elastic-plastic stresses in a rotating disk with von Mises’ yield criterion using general nonlinear strain hardening rule.

In this paper, thermal elastic-plastic stresses have been calculated for cylinder made up of functionally graded stainless steel composite material under internal and external pressure using finite difference method. In this problem, a general nonlinear strain hardening law with von Mises’ yield criterion has been considered. Results have been discussed numerically with the help of graphs and tables.

2. Objective

For a rotating cylinder with varying material properties, circumferential stress at the hub does not exceed the allow- able value which tells the designers little more than that the design of the cylinder is safe at the given pressure. Thus our prime objective is to calculate allowable thermal elastic- plastic stresses in an open ended functionally graded stainless steel composite rotating cylinder under pressure for varying expansion to incorporate a “safety factor” that prevents the cylinder from bursting under pressure and thermal loading.

3. Mathematical Formulation

3.1. Distribution of Material Properties. Consider a long open ended axisymmetric cylindermade up of functionally graded stainless steel composite material with inner and outer radii 𝑎 and 𝑏, respectively, and the cylinder is subjected to internal pressure 𝑝

𝑖 and external pressure 𝑝

0 as shown in Figure 1.

The cylindrical polar coordinates (𝑟, 𝜃) under plane stress condition have been considered in this problem.

In this study, Poisson’s ratio (]) and thermal expansion coefficient (𝛼 = 𝛼

0 ) are assumed to be constants. The

other properties, that is, Young’s modulus which is defined by power law, temperature distribution that follows Laplace

b r

a

𝜃 p0

pi

Figure 1: A functionally graded rotating cylinder with inner pressure 𝑝

𝑖 and outer pressure 𝑝

0 at the boundary.

heat equation in radial direction, thickness, and density, are varying radially and are expressed as

𝐸 (𝑟) = 𝐸0 (

𝑟

𝑏

)

𝑒 1

, 𝜃 (𝑟) = 𝜃0 log(𝑟

𝑏

) ,

𝜌 (𝑟) = 𝜌0 (

𝑟

𝑏

)

𝑑

, ℎ (𝑟) = ℎ0 (

𝑟

𝑏

)

−𝑙

,

(1)

where 𝜃 0 = 𝜃 0 /(log(𝑎/𝑏)), 𝑟 is the radius of the cylinder, 𝐸

0 ,

𝜌 0 , 𝜃 0 , and ℎ

0 are material constants, and 𝑒

1 , 𝑑, and 𝑙 are the

geometric parameters.

3.2. Basic Equations. The equilibrium equation for the cylin- der in the absence of body forces is

𝑑

𝑑𝑟

(ℎ𝑟𝑇 𝑟𝑟 ) − ℎ𝑇

𝜃𝜃 + ℎ𝜌𝜔

2 𝑟 2 = 0, (2)

where 𝑇 𝑟𝑟

and 𝑇 𝜃𝜃

are radial and circumferential stresses, respectively.

Using infinitesimal theory of elasticity, the relations between strains and radial displacements are

𝑒 𝑟 =

𝑑𝑢

𝑑𝑟

, 𝑒 𝜃 =

𝑢

𝑟

, (3)

where 𝑒 𝑟 and 𝑒

𝜃 are radial and circumferential strains,

respectively, and 𝑢 is the radial displacement. The equation of compatibility can be derived from (3) as

𝑑𝑒 𝜃

𝑑𝑟

+

𝑒 𝜃 − 𝑒 𝑟

𝑟

= 0. (4)

From infinitesimal theory of elasticity, the stress-strain relations are

𝑒 𝑒

𝑟 =

1

𝐸

[𝑇 𝑟𝑟 − ] (𝑇

𝜃𝜃 + 𝑇 𝑧𝑧 )] , 𝑒

𝑒

𝜃 =

1

𝐸

[𝑇 𝜃𝜃 − ] (𝑇

𝑟𝑟 + 𝑇 𝑧𝑧 )] ,

𝑒 𝑒

𝑧 =

1

𝐸

[𝑇 𝑧𝑧 − ] (𝑇

𝑟𝑟 + 𝑇 𝜃𝜃 )] ,

(5)

where 𝑒𝑒 𝑟 , 𝑒𝑒 𝜃 , and 𝑒𝑒

𝑧 are the elastic radial, circumferential, and

axial strains, respectively.

Advances in Materials Science and Engineering 3

*View more*